On microstructure-property relationships derived ... On microstructure-property relationships...
Embed Size (px)
Transcript of On microstructure-property relationships derived ... On microstructure-property relationships...
On microstructure-property relationships derived by virtual materials testing with an
emphasis on effective conductivity
Matthias Neumann1?, Orkun Furat1, Dzmitry Hlushkou2??, Ulrich Tallarek2??, Lorenz Holzer3, and Volker Schmidt1?
1 Institute of Stochastics, Ulm University, Helmholtzstraße 18, D-89069 Ulm, Germany
2 Department of Chemistry, Philipps-Universität Marburg, Hans-Meerwein-Straße 4, D-35032 Marburg, Germany
3 Institute of Computational Physics, ZHAW, Wildbachstrasse 21, CH-8400 Winterthur, Switzerland
Abstract. Based on virtual materials testing, which combines image analysis, stochastic microstructure modeling and numerical simulations, quantitative relationships between microstructure characteristics and ef- fective conductivity can be derived. The idea of virtual materials testing is to generate a large variety of stochastically simulated microstructures in short time. These virtual, but realistic microstructures are used as input for numerical transport simulations. Finally, a large data basis is available to study microstructure-property relationships quantitatively by classical regression analysis and tools from statistical learning. The microstructure-property relationships obtained for effective conductivity can also be applied to Fickian diffusion. For validation, we discuss an example of Fickian diffusion in porous silica monoliths on the basis of 3D image data.
The functionality of many materials, like, e.g., solar cells , batteries , fuel cells  or silica monoliths used for catalysis , is strongly influenced by their microstructure. Thus an optimal design of the microstructure regarding effec- tive macroscopic properties of these materials would lead to an improvement of their functionality. This kind of microstructure optimization, in turn, requires an understanding of the quantitative relationships between microstructure charac- teristics and effective macroscopic properties, which are – so far – only available for some special types of simple microstructures  like, e.g., the coated spheres model introduced in .
? The work of MN and VS has been partially funded by the German Federal Ministry for Economic Affairs and Energy (BMWi) under grant 03ET6095E.
?? The work of DH and UT has been supported by the Deutsche Forschungsgemein- schaft DFG (Bonn, Germany) under grant TA 268/9-1.
A direct approach to investigate relationships between microstructure and effective macroscopic properties is based on tomographic 3D imaging of mi- crostructures. Among other methods, X-ray tomography , FIB-SEM tomogra- phy  and STEM tomography  provide highly resolved information about mi- crostructures on different length scales. On the one hand, 3D image data can be analyzed by tools from spatial statistics  and mathematical morphology , which allows the computation of well-defined microstructure characteristics. On the other hand, 3D image data can be used as an input information for the nu- merical simulation of effective macroscopic properties, like, e.g., effective diffu- sivity in silica monoliths . This combination of image analysis and numerical simulation enables a direct investigation of the relationship between well-defined microstructure characteristics and effective macroscopic properties [12–16]. How- ever, this approach is limited as it is not possible to investigate a sufficiently large data set of different microstructures due to the high costs of 3D imaging.
Thus an alternative approach – called virtual materials testing – was sug- gested where image analysis and numerical simulations are combined with stochas- tic 3D microstructure modeling . By the aid of stochastic modeling virtual, but realistic, microstructures can be generated in short time. So a large data set of virtual microstructures with a wide range of microstructure character- istics is generated in order to study the quantitative relationship between mi- crostructure characteristics and effective macroscopic properties efficiently. In the present paper, we give an overview of the results having been obtained for the microstructure influence on electric conductivity by virtual materials test- ing [17–19]. Furthermore, we show how the results can be used to predict effective diffusivity in silica monoliths.
Before we give a detailed description on how to simulate the considered stochastic 3D microstructure model in Sect. 3, the microstructure characteristics which are related to effective conductivity are described in Sect. 2. The results of virtual materials testing with respect to electric conductivity are reviewed in Sect. 4. It is shown in Sect. 5 that the results can be used to predict effective diffusivity in silica monoliths the morphology of which has been analyzed in . Conclusions are given in Sect. 6.
2 Microstructure Characteristics and M -factor
To investigate the microstructure influence on effective conductivity σeff we con- sider the microstructure characteristics volume fraction ε, mean geometric tor- tuosity τgeom, mean geodesic tortuosity τgeod and constrictivity β. These mi- crostructure characteristics are computed based on voxelized 3D images repre- senting (virtual or real) microstructures. Moreover, using ε, τgeom, τgeod, β the M -factor
M = σeff/σ0 (1)
is predicted, where σ0 denotes the intrinsic conductivity of the considered ma- terial.
As described in , we consider conductive transport processes within porous materials with one conducting phase, the intrinsic conductivity of which is σ0.
Let J denote the current density, σ the space-dependent conductivity func- tion, U the electric potential and t the time. Then, electric charge transport is described by Ohm’s law
J = −σ∂U ∂x
∂t = σ
∂x2 . (3)
Assuming constant boundary conditions, such systems converge to an equilib- rium which is described by the Laplace equation
∆U = 0. (4)
By averaging over J and U as described in  we obtain the effective con- ductivity σeff and thus the M -factor of the microstructure. For the numerical simulation of M the software NM-SESES  has been used in , while Geo- Dict  has been used in [18,19].
Fig. 1. Visualization of two different kinds of shortest path corresponding to τgeom(center, right) and τgeod(left) in 2D. The conducting phase is represented in white, while sphericle obstacles are represented in grey. The shortest paths from the start layer to the goal layer are visualized in blue. The skeleton on which the paths for τgeom are computed is represented by a grey network (right).1
1 Reprinted from , Figure 3, with permission of J. Wiley & Sons.
Both characteristics, τgeom and τgeod describe the length of paths through the conducting phase relative to the thickness of the material. Note that – in con- trast to concepts of effective tortuosity – the characteristics τgeom and τgeod depend only on the geometry of the microstructure. An overview on the avail- able concepts of tortuosity in the literature is given in . To determine τgeod, we compute for each voxel of the conducting phase located at the start layer, i.e. the plane where the conduction process starts, the shortest path through the conducting phase to the goal layer in terms of geodesic distance . Such a shortest path is visualized in Fig. 1(left). Mean geodesic tortuosity τgeod is defined as the average of these path lengths divided by the thickness of the ma- terial. Mean geometric tortuosity τgeom is also defined as an average of shortest path lengths, where shortest paths are computed on a skeleton of the conducting phase, see Fig. 1(right). The skeleton of a microstructure is a network of medial axes through the conducting phase . In  and  the software Avizo  has been used to extract the skeleton from 3D image data.
Constrictivity β quantifies bottleneck effects. It has been defined for a single tube with periodic constrictions in  by β = (rmin/rmax)
2, where rmin and rmax are the radius of the minimum and maximum cross-section of the tube, respectively. This concept of constrictivity has been generalized defining rmin, rmax and thus β for complex microstructures . As described in , rmax is defined as the 50% quantile of the continuous pore size distribution, while rmin is defined as the 50% quantile of the MIP pore size distribution, which is based on a geometrical simulation of mercury intrusion porosimetry, introduced in . Constrictivity takes values between 0 and 1, where values close to 0 indicate strong bottleneck effects while values close to 1 indicate that there are no bottlenecks at all.
3 Stochastic 3D Microstructure Model
In , a parametric stochastic 3D microstructure model has been developed, which has been used to simulate virtual microstructures with many different constellations for the microstructure characteristics ε, τgeom (or τgeod) and β. We recall the definition of the model introduced in  and give a detailed description on how to simulate model realizations.
3.1 Model Definition
Using tools of stochastic geometry and graph theory, we define a random set Ξ representing the conducting phase of a microstructure. At first a random geometric graph G = (V,E) is modeled consisting of a set of vertices V and a set of edges E, which are connections between the vertices. In a second step the
Fig. 2. Generalized RNG, where the set of vertices is given by a reali